#------------------------------------------------------------------------------
#$Date: 2016-02-16 22:30:59 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176467 $
#$URL: svn://www.crystallography.net/cod/cif/4/30/85/4308524.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4308524
loop_
_publ_author_name
'Feng He'
'Ming-Liang Tong'
'Xiao-Lan Yu'
'Xiao-Ming Chen'
_publ_contact_author
;
      Chen, Xiao-Ming
      School of Chemistry and Chemical Engineering
      Sun Yat-Sen University
      Guangzhou, 510275
      P. R. China
;
_publ_contact_author_email       cescxm@zsu.edu.cn
_publ_contact_author_fax         '86 20 84112245'
_publ_contact_author_phone       86-20-84113986
_publ_section_title
;
Controlled Aggregation of Heterometallic Nanoscale Cu12Ln6 Clusters (Ln =
GdIII or NdIII) into 2D Coordination Polymers
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              559
_journal_page_last               565
_journal_paper_doi               10.1021/ic048754s
_journal_volume                  44
_journal_year                    2005
_chemical_formula_sum            'C36 H116 Cl0.5 Cu16 N57.5 Nd6 O106.5'
_chemical_formula_weight         4958.67
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           87
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4'
_symmetry_space_group_name_H-M   'I 4/m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   20.4620(6)
_cell_length_b                   20.4620(6)
_cell_length_c                   18.9592(10)
_cell_measurement_temperature    295(2)
_cell_volume                     7938.1(5)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      295(2)
_diffrn_measured_fraction_theta_full 0.961
_diffrn_measured_fraction_theta_max 0.961
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0312
_diffrn_reflns_av_sigmaI/netI    0.0257
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -26
_diffrn_reflns_limit_k_max       26
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_limit_l_min       -25
_diffrn_reflns_number            25000
_diffrn_reflns_theta_full        28.31
_diffrn_reflns_theta_max         28.31
_diffrn_reflns_theta_min         1.41
_exptl_absorpt_coefficient_mu    4.144
_exptl_crystal_colour            blue
_exptl_crystal_density_diffrn    2.075
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             4838
_exptl_crystal_size_max          0.24
_exptl_crystal_size_mid          0.21
_exptl_crystal_size_min          0.14
_refine_diff_density_max         1.750
_refine_diff_density_min         -2.034
_refine_diff_density_rms         0.249
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.318
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     291
_refine_ls_number_reflns         4891
_refine_ls_number_restraints     337
_refine_ls_restrained_S_all      1.300
_refine_ls_R_factor_all          0.0908
_refine_ls_R_factor_gt           0.0894
_refine_ls_shift/su_max          1.791
_refine_ls_shift/su_mean         0.019
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0708P)²+283.1898P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2102
_refine_ls_wR_factor_ref         0.2111
_reflns_number_gt                4820
_reflns_number_total             4891
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic048754ssi20040906_102134_1.cif
_cod_data_source_block           compoud_2Nd
_cod_original_formula_sum        'C36 H116 Cl0.50 Cu16 Nd6 N57.50 O106.50'
_cod_database_code               4308524
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-y, x, z'
'y, -x, z'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'-y+1/2, x+1/2, z+1/2'
'y+1/2, -x+1/2, z+1/2'
'-x, -y, -z'
'x, y, -z'
'y, -x, -z'
'-y, x, -z'
'-x+1/2, -y+1/2, -z+1/2'
'x+1/2, y+1/2, -z+1/2'
'y+1/2, -x+1/2, -z+1/2'
'-y+1/2, x+1/2, -z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Nd1 Nd 0.08805(3) 0.22788(3) 0.0000 0.0194(2) Uani 1 2 d SU . .
Nd2 Nd 0.0000 0.0000 -0.26811(5) 0.0233(2) Uani 1 4 d SU . .
Cu1 Cu 0.04158(5) 0.10950(5) -0.12841(6) 0.0226(3) Uani 1 1 d U . .
Cu2 Cu 0.15149(8) 0.06764(7) 0.0000 0.0220(3) Uani 1 2 d SU . .
Cu3 Cu 0.0000 0.5000 -0.07577(12) 0.0466(6) Uani 1 2 d SU . .
Cl1 Cl 0.0000 0.0000 0.0000 0.038(2) Uani 0.50 8 d SPU . .
N01 N 0.0000 0.0000 0.0000 0.038(2) Uani 0.50 8 d SPDU . .
O01 O 0.0000 0.0000 0.0648(5) 0.018(6) Uani 0.25 4 d SPDU . .
O02 O 0.0428(15) 0.020(2) -0.0400(14) 0.018(6) Uani 0.13 1 d PDU . .
O1H O 0.0849(3) 0.0371(3) -0.1816(4) 0.0231(13) Uani 1 1 d U . .
H1HA H 0.1230 0.0540 -0.2074 0.028 Uiso 1 1 d R . .
O2H O 0.1178(3) 0.1283(3) -0.0707(3) 0.0229(13) Uani 1 1 d U . .
H2HA H 0.1540 0.1405 -0.1023 0.027 Uiso 1 1 d R . .
O3H O -0.0029(3) 0.1777(3) -0.0707(3) 0.0228(13) Uani 1 1 d U . .
H3HA H -0.0217 0.2112 -0.1020 0.027 Uiso 1 1 d R . .
O4H O 0.0250(5) 0.4417(5) 0.0000 0.034(2) Uani 1 2 d SU . .
H4HA H 0.0659 0.4336 0.0000 0.041 Uiso 1 2 d SR . .
O1W O -0.0029(5) 0.3103(5) 0.0000 0.034(2) Uani 1 2 d SU . .
H1WA H -0.0468 0.3056 0.0000 0.041 Uiso 1 2 d SR . .
H1WB H 0.0094 0.3526 0.0000 0.041 Uiso 1 2 d SR . .
O2W O 0.1338(6) 0.3442(5) 0.0000 0.043(3) Uani 1 2 d SU . .
H2W H 0.1562 0.3598 0.0369 0.051 Uiso 1 1 d R . .
O3W O 0.1065(4) -0.0422(5) -0.3132(5) 0.048(2) Uani 1 1 d U . .
H3WB H 0.1294 -0.0157 -0.3377 0.058 Uiso 1 1 d R . .
H3WC H 0.1060 -0.0809 -0.3300 0.058 Uiso 1 1 d R . .
O4W O 0.0000 0.0000 -0.3993(9) 0.044(4) Uani 1 4 d SU . .
H4WA H -0.0140 -0.0367 -0.4144 0.066 Uiso 0.50 1 d PR . .
C1 C 0.0878(5) 0.2453(5) -0.1849(6) 0.031(2) Uani 1 1 d U . .
C2 C 0.0791(7) 0.2972(6) -0.2412(6) 0.040(3) Uani 1 1 d U . .
H2A H 0.1169 0.2973 -0.2721 0.048 Uiso 1 1 calc R . .
H2B H 0.0410 0.2869 -0.2696 0.048 Uiso 1 1 calc R . .
N1 N 0.0712(5) 0.3614(4) -0.2101(5) 0.0332(19) Uani 1 1 d U . .
N2 N 0.1073(7) 0.4122(6) -0.2297(7) 0.060(3) Uani 1 1 d U . .
N3 N 0.0872(7) 0.4612(6) -0.1927(7) 0.063(3) Uani 1 1 d U . .
N4 N 0.0399(5) 0.4426(5) -0.1484(5) 0.042(2) Uani 1 1 d U . .
C3 C 0.0311(6) 0.3801(6) -0.1613(6) 0.040(3) Uani 1 1 d U . .
H3A H 0.0007 0.3535 -0.1389 0.048 Uiso 1 1 calc R . .
O1 O 0.1002(4) 0.2632(3) -0.1239(4) 0.0312(15) Uani 1 1 d U . .
O2 O 0.0814(5) 0.1878(4) -0.2070(4) 0.044(2) Uani 1 1 d U . .
O3 O 0.2534(6) 0.1248(6) 0.0000 0.042(3) Uani 1 2 d SU . .
O4 O 0.2069(5) 0.2237(6) 0.0000 0.043(3) Uani 1 2 d SU . .
N5 N 0.4467(9) 0.1102(10) 0.0391(11) 0.106(6) Uani 1 1 d U . .
C4 C 0.2540(9) 0.1849(9) 0.0000 0.046(4) Uani 1 2 d SU . .
C5 C 0.3164(18) 0.2208(19) 0.0000 0.120(12) Uani 1 2 d SU . .
H5 H 0.3183 0.2486 0.0411 0.144 Uiso 1 1 d R . .
N6 N 0.3759(14) 0.1776(14) 0.0000 0.099(8) Uani 1 2 d SU . .
C7 C 0.3974(16) 0.1475(16) 0.0626(17) 0.152(11) Uani 0.50 1 d PU . .
N7 N 0.3974(16) 0.1475(16) 0.0626(17) 0.152(11) Uani 0.50 1 d PU . .
H7 H 0.3791 0.1521 0.1093 0.183 Uiso 0.50 1 d PR . .
N8 N 0.2353(13) 0.1117(12) -0.2037(13) 0.217(16) Uani 1 1 d DU . .
O13 O 0.2034(17) 0.0871(16) -0.2556(15) 0.129(9) Uani 0.55 1 d PDU . .
O14 O 0.2608(16) 0.0705(17) -0.1585(16) 0.130(9) Uani 0.55 1 d PDU . .
O15 O 0.241(3) 0.1722(13) -0.192(3) 0.34(3) Uani 0.55 1 d PDU . .
O13' O 0.252(2) 0.1558(17) -0.2514(18) 0.129(9) Uani 0.45 1 d PDU . .
O14' O 0.247(2) 0.124(2) -0.1406(14) 0.130(9) Uani 0.45 1 d PDU . .
O15' O 0.222(6) 0.054(2) -0.225(3) 0.34(3) Uani 0.45 1 d PDU . .
N9 N 0.370(8) 0.568(7) 0.0000 0.21(8) Uani 0.25 2 d SPDU . .
O16 O 0.408(5) 0.521(4) 0.0000 0.12(3) Uiso 0.25 2 d SPD . .
O17 O 0.349(4) 0.599(3) -0.0507(16) 0.13(2) Uiso 0.25 1 d PD . .
O5W O 0.2233(17) 0.3859(17) 0.0972(19) 0.260(16) Uani 1 1 d U . .
H5WA H 0.2059 0.3991 0.1357 0.311 Uiso 1 1 d R . .
H5WB H 0.2488 0.3540 0.1059 0.311 Uiso 1 1 d R . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nd Nd -0.1943 3.0179 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O4 Nd1 O1 84.80(19) . 10 ?
O4 Nd1 O1 84.80(19) . . ?
O1 Nd1 O1 144.0(3) 10 . ?
O4 Nd1 O1W 139.8(4) . . ?
O1 Nd1 O1W 83.04(19) 10 . ?
O1 Nd1 O1W 83.04(19) . . ?
O4 Nd1 O3H 136.6(2) . . ?
O1 Nd1 O3H 134.5(2) 10 . ?
O1 Nd1 O3H 71.8(2) . . ?
O1W Nd1 O3H 74.0(2) . . ?
O4 Nd1 O3H 136.6(2) . 10 ?
O1 Nd1 O3H 71.8(2) 10 10 ?
O1 Nd1 O3H 134.5(2) . 10 ?
O1W Nd1 O3H 74.0(2) . 10 ?
O3H Nd1 O3H 64.4(3) . 10 ?
O4 Nd1 O2H 74.3(3) . . ?
O1 Nd1 O2H 136.0(2) 10 . ?
O1 Nd1 O2H 72.8(2) . . ?
O1W Nd1 O2H 136.3(2) . . ?
O3H Nd1 O2H 64.1(2) . . ?
O3H Nd1 O2H 97.6(2) 10 . ?
O4 Nd1 O2H 74.3(3) . 10 ?
O1 Nd1 O2H 72.8(2) 10 10 ?
O1 Nd1 O2H 136.0(2) . 10 ?
O1W Nd1 O2H 136.3(2) . 10 ?
O3H Nd1 O2H 97.6(2) . 10 ?
O3H Nd1 O2H 64.1(2) 10 10 ?
O2H Nd1 O2H 64.5(3) . 10 ?
O4 Nd1 O2W 70.5(4) . . ?
O1 Nd1 O2W 72.01(16) 10 . ?
O1 Nd1 O2W 72.01(16) . . ?
O1W Nd1 O2W 69.3(4) . . ?
O3H Nd1 O2W 130.7(2) . . ?
O3H Nd1 O2W 130.7(2) 10 . ?
O2H Nd1 O2W 131.7(2) . . ?
O2H Nd1 O2W 131.7(2) 10 . ?
O4 Nd1 Cu2 66.4(3) . . ?
O1 Nd1 Cu2 103.56(17) 10 . ?
O1 Nd1 Cu2 103.56(17) . . ?
O1W Nd1 Cu2 153.8(2) . . ?
O3H Nd1 Cu2 83.84(15) . . ?
O3H Nd1 Cu2 83.84(15) 10 . ?
O2H Nd1 Cu2 32.57(15) . . ?
O2H Nd1 Cu2 32.57(15) 10 . ?
O2W Nd1 Cu2 136.9(3) . . ?
O4 Nd1 Cu2 151.9(3) . 3 ?
O1 Nd1 Cu2 102.67(17) 10 3 ?
O1 Nd1 Cu2 102.67(17) . 3 ?
O1W Nd1 Cu2 68.3(2) . 3 ?
O3H Nd1 Cu2 32.32(15) . 3 ?
O3H Nd1 Cu2 32.32(15) 10 3 ?
O2H Nd1 Cu2 81.97(15) . 3 ?
O2H Nd1 Cu2 81.97(15) 10 3 ?
O2W Nd1 Cu2 137.6(3) . 3 ?
Cu2 Nd1 Cu2 85.46(5) . 3 ?
O4 Nd1 Cu1 104.06(19) . . ?
O1 Nd1 Cu1 151.08(17) 10 . ?
O1 Nd1 Cu1 64.90(16) . . ?
O1W Nd1 Cu1 104.98(17) . . ?
O3H Nd1 Cu1 32.90(15) . . ?
O3H Nd1 Cu1 83.61(15) 10 . ?
O2H Nd1 Cu1 31.71(15) . . ?
O2H Nd1 Cu1 83.00(15) 10 . ?
O2W Nd1 Cu1 136.91(2) . . ?
Cu2 Nd1 Cu1 57.74(3) . . ?
Cu2 Nd1 Cu1 57.38(3) 3 . ?
O4W Nd2 O3W 70.0(2) . 4 ?
O4W Nd2 O3W 70.0(2) . 2 ?
O3W Nd2 O3W 83.27(14) 4 2 ?
O4W Nd2 O3W 70.0(2) . 3 ?
O3W Nd2 O3W 140.0(4) 4 3 ?
O3W Nd2 O3W 83.27(14) 2 3 ?
O4W Nd2 O3W 70.0(2) . . ?
O3W Nd2 O3W 83.27(14) 4 . ?
O3W Nd2 O3W 140.0(4) 2 . ?
O3W Nd2 O3W 83.27(14) 3 . ?
O4W Nd2 O1H 130.87(15) . 3 ?
O3W Nd2 O1H 136.4(3) 4 3 ?
O3W Nd2 O1H 73.7(3) 2 3 ?
O3W Nd2 O1H 74.0(3) 3 3 ?
O3W Nd2 O1H 136.8(3) . 3 ?
O4W Nd2 O1H 130.87(15) . . ?
O3W Nd2 O1H 136.8(3) 4 . ?
O3W Nd2 O1H 136.4(3) 2 . ?
O3W Nd2 O1H 73.7(3) 3 . ?
O3W Nd2 O1H 74.0(3) . . ?
O1H Nd2 O1H 64.65(17) 3 . ?
O4W Nd2 O1H 130.87(15) . 4 ?
O3W Nd2 O1H 74.0(3) 4 4 ?
O3W Nd2 O1H 136.8(3) 2 4 ?
O3W Nd2 O1H 136.4(3) 3 4 ?
O3W Nd2 O1H 73.7(3) . 4 ?
O1H Nd2 O1H 98.3(3) 3 4 ?
O1H Nd2 O1H 64.65(17) . 4 ?
O4W Nd2 O1H 130.87(15) . 2 ?
O3W Nd2 O1H 73.7(3) 4 2 ?
O3W Nd2 O1H 74.0(3) 2 2 ?
O3W Nd2 O1H 136.8(3) 3 2 ?
O3W Nd2 O1H 136.4(3) . 2 ?
O1H Nd2 O1H 64.65(17) 3 2 ?
O1H Nd2 O1H 98.3(3) . 2 ?
O1H Nd2 O1H 64.65(17) 4 2 ?
O4W Nd2 Cu1 137.86(2) . . ?
O3W Nd2 Cu1 152.2(2) 4 . ?
O3W Nd2 Cu1 104.2(2) 2 . ?
O3W Nd2 Cu1 67.9(2) 3 . ?
O3W Nd2 Cu1 105.2(2) . . ?
O1H Nd2 Cu1 32.05(14) 3 . ?
O1H Nd2 Cu1 32.83(14) . . ?
O1H Nd2 Cu1 82.95(15) 4 . ?
O1H Nd2 Cu1 82.52(15) 2 . ?
O4W Nd2 Cu1 137.86(2) . 4 ?
O3W Nd2 Cu1 105.2(2) 4 4 ?
O3W Nd2 Cu1 152.2(2) 2 4 ?
O3W Nd2 Cu1 104.2(2) 3 4 ?
O3W Nd2 Cu1 67.9(2) . 4 ?
O1H Nd2 Cu1 82.52(15) 3 4 ?
O1H Nd2 Cu1 32.05(14) . 4 ?
O1H Nd2 Cu1 32.83(14) 4 4 ?
O1H Nd2 Cu1 82.95(15) 2 4 ?
Cu1 Nd2 Cu1 56.64(2) . 4 ?
O4W Nd2 Cu1 137.86(2) . 2 ?
O3W Nd2 Cu1 67.9(2) 4 2 ?
O3W Nd2 Cu1 105.2(2) 2 2 ?
O3W Nd2 Cu1 152.2(2) 3 2 ?
O3W Nd2 Cu1 104.2(2) . 2 ?
O1H Nd2 Cu1 82.95(15) 3 2 ?
O1H Nd2 Cu1 82.52(15) . 2 ?
O1H Nd2 Cu1 32.05(14) 4 2 ?
O1H Nd2 Cu1 32.83(14) 2 2 ?
Cu1 Nd2 Cu1 84.28(4) . 2 ?
Cu1 Nd2 Cu1 56.65(2) 4 2 ?
O2H Cu1 O1H 175.5(3) . 3 ?
O2H Cu1 O3H 85.3(3) . . ?
O1H Cu1 O3H 95.0(3) 3 . ?
O2H Cu1 O1H 94.3(3) . . ?
O1H Cu1 O1H 85.1(4) 3 . ?
O3H Cu1 O1H 176.4(3) . . ?
O2H Cu1 O2 86.8(3) . . ?
O1H Cu1 O2 97.7(3) 3 . ?
O3H Cu1 O2 91.7(3) . . ?
O1H Cu1 O2 91.8(3) . . ?
O2H Cu1 Nd1 42.85(18) . . ?
O1H Cu1 Nd1 137.99(19) 3 . ?
O3H Cu1 Nd1 43.19(18) . . ?
O1H Cu1 Nd1 136.87(19) . . ?
O2 Cu1 Nd1 82.9(2) . . ?
O2H Cu1 Nd2 137.11(19) . . ?
O1H Cu1 Nd2 42.61(19) 3 . ?
O3H Cu1 Nd2 137.52(19) . . ?
O1H Cu1 Nd2 42.86(19) . . ?
O2 Cu1 Nd2 92.3(2) . . ?
Nd1 Cu1 Nd2 175.21(4) . . ?
O2H Cu2 O2H 86.7(4) 10 . ?
O2H Cu2 O3H 93.3(3) 10 11 ?
O2H Cu2 O3H 174.9(3) . 11 ?
O2H Cu2 O3H 174.9(3) 10 4 ?
O2H Cu2 O3H 93.3(3) . 4 ?
O3H Cu2 O3H 86.3(4) 11 4 ?
O2H Cu2 O3 89.8(3) 10 . ?
O2H Cu2 O3 89.8(3) . . ?
O3H Cu2 O3 95.3(3) 11 . ?
O3H Cu2 O3 95.3(3) 4 . ?
O2H Cu2 Nd1 43.87(19) 10 . ?
O2H Cu2 Nd1 43.87(19) . . ?
O3H Cu2 Nd1 136.84(19) 11 . ?
O3H Cu2 Nd1 136.84(19) 4 . ?
O3 Cu2 Nd1 82.3(3) . . ?
O2H Cu2 Nd1 136.56(19) 10 11 ?
O2H Cu2 Nd1 136.56(19) . 11 ?
O3H Cu2 Nd1 43.31(19) 11 11 ?
O3H Cu2 Nd1 43.31(19) 4 11 ?
O3 Cu2 Nd1 93.1(3) . 11 ?
Nd1 Cu2 Nd1 175.46(5) . 11 ?
O4H Cu3 O4H 84.2(5) 9_565 . ?
O4H Cu3 N4 171.0(5) 9_565 . ?
O4H Cu3 N4 92.4(4) . . ?
O4H Cu3 N4 92.4(4) 9_565 2_565 ?
O4H Cu3 N4 171.0(5) . 2_565 ?
N4 Cu3 N4 92.2(6) . 2_565 ?
O4H Cu3 Cu3 42.1(2) 9_565 9_565 ?
O4H Cu3 Cu3 42.1(2) . 9_565 ?
N4 Cu3 Cu3 133.9(3) . 9_565 ?
N4 Cu3 Cu3 133.9(3) 2_565 9_565 ?
O01 Cl1 O01 180.0 . 9 ?
O01 Cl1 O02 52.0(16) . 10 ?
O01 Cl1 O02 128.0(16) 9 10 ?
O01 Cl1 O02 52.0(16) . 12 ?
O01 Cl1 O02 128.0(16) 9 12 ?
O02 Cl1 O02 67.8(17) 10 12 ?
O01 Cl1 O02 52.0(16) . 11 ?
O01 Cl1 O02 128.0(16) 9 11 ?
O02 Cl1 O02 67.8(17) 10 11 ?
O02 Cl1 O02 104(3) 12 11 ?
O01 Cl1 O02 52.0(16) . 9 ?
O01 Cl1 O02 128.0(16) 9 9 ?
O02 Cl1 O02 104(3) 10 9 ?
O02 Cl1 O02 67.8(17) 12 9 ?
O02 Cl1 O02 67.8(17) 11 9 ?
O01 Cl1 O02 128.0(16) . . ?
O01 Cl1 O02 52.0(16) 9 . ?
O02 Cl1 O02 76(3) 10 . ?
O02 Cl1 O02 112.2(17) 12 . ?
O02 Cl1 O02 112.2(17) 11 . ?
O02 Cl1 O02 180(3) 9 . ?
O01 Cl1 O02 128.0(16) . 2 ?
O01 Cl1 O02 52.0(16) 9 2 ?
O02 Cl1 O02 180(3) 10 2 ?
O02 Cl1 O02 112.2(17) 12 2 ?
O02 Cl1 O02 112.2(17) 11 2 ?
O02 Cl1 O02 76(3) 9 2 ?
O02 Cl1 O02 104(3) . 2 ?
O01 Cl1 O02 128.0(16) . 4 ?
O01 Cl1 O02 52.0(16) 9 4 ?
O02 Cl1 O02 112.2(17) 10 4 ?
O02 Cl1 O02 180(3) 12 4 ?
O02 Cl1 O02 76(3) 11 4 ?
O02 Cl1 O02 112.2(17) 9 4 ?
O02 Cl1 O02 67.8(17) . 4 ?
O02 Cl1 O02 67.8(17) 2 4 ?
O01 Cl1 O02 128.0(16) . 3 ?
O01 Cl1 O02 52.0(16) 9 3 ?
O02 Cl1 O02 112.2(17) 10 3 ?
O02 Cl1 O02 76(3) 12 3 ?
O02 Cl1 O02 180(3) 11 3 ?
O02 Cl1 O02 112.2(17) 9 3 ?
O02 Cl1 O02 67.8(17) . 3 ?
O02 Cl1 O02 67.8(17) 2 3 ?
O02 Cl1 O02 104(3) 4 3 ?
O02 O01 O02 128(2) 9 10 ?
O02 O01 O02 79.0(8) 9 11 ?
O02 O01 O02 79.0(8) 10 11 ?
O02 O01 O02 79.0(8) 9 12 ?
O02 O01 O02 79.0(8) 10 12 ?
O02 O01 O02 128(2) 11 12 ?
O02 O01 Cl1 64.2(11) 9 . ?
O02 O01 Cl1 64.2(11) 10 . ?
O02 O01 Cl1 64.2(11) 11 . ?
O02 O01 Cl1 64.2(11) 12 . ?
O01 O02 Cl1 63.8(11) 9 . ?
O01 O02 O02 50.5(4) 9 4 ?
Cl1 O02 O02 56.1(8) . 4 ?
O01 O02 O02 50.5(4) 9 3 ?
Cl1 O02 O02 56.1(9) . 3 ?
O02 O02 O02 90.000(6) 4 3 ?
O01 O02 O02 115.8(11) 9 10 ?
Cl1 O02 O02 52.0(16) . 10 ?
O02 O02 O02 90.000(3) 4 10 ?
O02 O02 O02 90.000(6) 3 10 ?
Cu1 O1H Cu1 117.5(3) 4 . ?
Cu1 O1H Nd2 105.3(3) 4 . ?
Cu1 O1H Nd2 104.3(3) . . ?
Cu1 O2H Cu2 122.9(3) . . ?
Cu1 O2H Nd1 105.4(3) . . ?
Cu2 O2H Nd1 103.6(3) . . ?
Cu2 O3H Cu1 119.5(3) 3 . ?
Cu2 O3H Nd1 104.4(3) 3 . ?
Cu1 O3H Nd1 103.9(3) . . ?
Cu3 O4H Cu3 95.8(5) 9_565 . ?
O1 C1 O2 127.6(10) . . ?
O1 C1 C2 118.3(9) . . ?
O2 C1 C2 114.1(10) . . ?
N1 C2 C1 111.2(10) . . ?
C3 N1 N2 108.6(10) . . ?
C3 N1 C2 129.0(10) . . ?
N2 N1 C2 122.3(10) . . ?
N3 N2 N1 106.3(11) . . ?
N2 N3 N4 110.5(11) . . ?
C3 N4 N3 105.0(10) . . ?
C3 N4 Cu3 130.4(9) . . ?
N3 N4 Cu3 124.5(8) . . ?
N1 C3 N4 109.5(11) . . ?
C1 O1 Nd1 141.3(6) . . ?
C1 O2 Cu1 117.8(7) . . ?
C4 O3 Cu2 119.8(11) . . ?
C4 O4 Nd1 142.5(11) . . ?
C7 N5 N5 109.4(17) . 10 ?
O3 C4 O4 128.9(17) . . ?
O3 C4 C5 121(2) . . ?
O4 C4 C5 111(2) . . ?
C4 C5 N6 114(3) . . ?
C7 N6 N7 115(3) . 10 ?
C7 N6 C7 115(3) . 10 ?
N7 N6 C7 0(4) 10 10 ?
C7 N6 C5 120.6(18) . . ?
N7 N6 C5 120.6(18) 10 . ?
C7 N6 C5 120.6(18) 10 . ?
N5 C7 N6 102(3) . . ?
O14' N8 O15 67(2) . . ?
O14' N8 O15' 122(2) . . ?
O15 N8 O15' 169(4) . . ?
O14' N8 O13 156(3) . . ?
O15 N8 O13 124.4(19) . . ?
O15' N8 O13 44(4) . . ?
O14' N8 O14 55(2) . . ?
O15 N8 O14 118.7(18) . . ?
O15' N8 O14 72(4) . . ?
O13 N8 O14 116.9(17) . . ?
O14' N8 O13' 117.6(18) . . ?
O15 N8 O13' 55(3) . . ?
O15' N8 O13' 118.2(19) . . ?
O13 N8 O13' 83(2) . . ?
O14 N8 O13' 141(3) . . ?
O15' O13 N8 67(2) . . ?
O15' O13 O13' 108(5) . . ?
N8 O13 O13' 49.5(13) . . ?
O14' O14 N8 59.6(14) . . ?
O14' O14 O15' 108(4) . . ?
N8 O14 O15' 52.5(19) . . ?
O13' O15 N8 65.3(19) . . ?
O13' O15 O14' 117(3) . . ?
N8 O15 O14' 55.9(14) . . ?
O15 O13' N8 60.0(16) . . ?
O15 O13' O13 99(3) . . ?
N8 O13' O13 47.5(13) . . ?
O14 O14' N8 64.9(16) . . ?
O14 O14' O15 118(2) . . ?
N8 O14' O15 56.9(15) . . ?
O13 O15' N8 69(2) . . ?
O13 O15' O14 124(2) . . ?
N8 O15' O14 55.0(19) . . ?
O16 N9 O17 128(3) . 10 ?
O16 N9 O17 128(3) . . ?
O17 N9 O17 103(5) 10 . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Nd1 O4 2.433(11) . ?
Nd1 O1 2.471(7) 10 ?
Nd1 O1 2.471(7) . ?
Nd1 O1W 2.511(10) . ?
Nd1 O3H 2.513(6) . ?
Nd1 O3H 2.513(6) 10 ?
Nd1 O2H 2.514(6) . ?
Nd1 O2H 2.514(6) 10 ?
Nd1 O2W 2.559(11) . ?
Nd1 Cu2 3.5266(16) . ?
Nd1 Cu2 3.5485(16) 3 ?
Nd1 Cu1 3.5636(12) . ?
Nd2 O4W 2.488(16) . ?
Nd2 O3W 2.495(8) 4 ?
Nd2 O3W 2.495(8) 2 ?
Nd2 O3W 2.495(8) 3 ?
Nd2 O3W 2.495(8) . ?
Nd2 O1H 2.508(7) 3 ?
Nd2 O1H 2.508(7) . ?
Nd2 O1H 2.508(7) 4 ?
Nd2 O1H 2.508(7) 2 ?
Nd2 Cu1 3.5720(13) . ?
Nd2 Cu1 3.5720(13) 4 ?
Nd2 Cu1 3.5720(13) 2 ?
Cu1 O2H 1.943(7) . ?
Cu1 O1H 1.965(6) 3 ?
Cu1 O3H 1.994(7) . ?
Cu1 O1H 1.999(6) . ?
Cu1 O2 2.335(8) . ?
Cu2 O2H 1.953(6) 10 ?
Cu2 O2H 1.953(6) . ?
Cu2 O3H 1.958(6) 11 ?
Cu2 O3H 1.958(6) 4 ?
Cu2 O3 2.391(12) . ?
Cu2 Nd1 3.5485(16) 11 ?
Cu3 O4H 1.936(7) 9_565 ?
Cu3 O4H 1.936(7) . ?
Cu3 N4 1.985(10) . ?
Cu3 N4 1.985(10) 2_565 ?
Cu3 Cu3 2.873(4) 9_565 ?
Cl1 O01 1.228(10) . ?
Cl1 O01 1.228(10) 9 ?
Cl1 O02 1.232(10) 10 ?
Cl1 O02 1.232(10) 12 ?
Cl1 O02 1.232(10) 11 ?
Cl1 O02 1.232(10) 9 ?
Cl1 O02 1.232(10) . ?
Cl1 O02 1.232(10) 2 ?
Cl1 O02 1.232(10) 4 ?
Cl1 O02 1.232(10) 3 ?
O01 O02 1.08(3) 9 ?
O01 O02 1.08(3) 10 ?
O01 O02 1.08(3) 11 ?
O01 O02 1.08(3) 12 ?
O02 O01 1.08(3) 9 ?
O02 O02 1.37(3) 4 ?
O02 O02 1.37(3) 3 ?
O02 O02 1.52(5) 10 ?
O1H Cu1 1.965(6) 4 ?
O3H Cu2 1.958(6) 3 ?
O4H Cu3 1.936(7) 9_565 ?
C1 O1 1.239(13) . ?
C1 O2 1.256(13) . ?
C1 C2 1.517(15) . ?
C2 N1 1.448(14) . ?
N1 C3 1.296(15) . ?
N1 N2 1.328(14) . ?
N2 N3 1.290(17) . ?
N3 N4 1.337(16) . ?
N4 C3 1.316(15) . ?
O3 C4 1.23(2) . ?
O4 C4 1.25(2) . ?
N5 C7 1.34(3) . ?
N5 N5 1.48(4) 10 ?
C4 C5 1.47(4) . ?
C5 N6 1.51(4) . ?
N6 C7 1.41(3) . ?
N6 N7 1.41(3) 10 ?
N6 C7 1.41(3) 10 ?
N8 O14' 1.248(17) . ?
N8 O15 1.264(16) . ?
N8 O15' 1.268(17) . ?
N8 O13 1.283(16) . ?
N8 O14 1.310(17) . ?
N8 O13' 1.325(17) . ?
O13 O15' 0.96(8) . ?
O13 O13' 1.73(4) . ?
O14 O14' 1.19(4) . ?
O14 O15' 1.52(6) . ?
O15 O13' 1.19(6) . ?
O15 O14' 1.39(4) . ?
N9 O16 1.240(12) . ?
N9 O17 1.226(12) 10 ?
N9 O17 1.226(12) . ?
